Discussion Chain ID: 138726
================================================================================

User asked: Do we have some "rule of thumb" to estimate the miscibility of metals?

For example, for ordinary fluids, we have polar and apolar ones. The "rule of thumb" is that polar fluids mix with each other, and also apolar fluids mix with each other, but polar fluids don't mix with apolars. Of course, it is not a very exact rule. For example, bensene mixes in water - but it does it badly. While the also polar ethanol mixes water very well. What is the case with liquid metals? Does some analogous - possibly more complex - category structure exist?

Discussion:
Comment: Most liquid metals mix with each other. Cases of non-miscibility are rare.
Comment: @IvanNeretin Thanks! But, for example, molten uranium does not mix with molten iron. Iron does not mix with gold. And so on.
Comment: @IvanNeretin - rare, perhaps, but common enough once you've seen enough phase diagrams. Lead in particular is prone to miscibility gaps. Then you get some weird things like Ag-Cu has a eutectic, Cu-Ni is mainly completely soluble (with a solid miscibility gap at low temperatures), but Ag-Ni has a huge liquid miscibility gap that only disappears around 3000K. And all are fcc metals. So, no, there is no 'rule of thumb' that works.
Comment: @NilayGhosh Amalgams are a specific form of mixtures, i.e. when one of the parts is mercury. It is a sub-set of the question, i.e. if we would only see the miscibility of only the water with other liquids. The "rule of thumb" I described, would work: polar liquids mostly mix with water, apolar ones don't.
Comment: https://chemistry.stackexchange.com/questions/35014/miscibility-of-molten-metals https://chemistry.stackexchange.com/questions/42248/why-are-pd-and-pt-completely-soluble-in-cu-but-ag-only-partly-in-cu-when-formin

Answer 1 (11 votes):
Bottom line: there are no simple rules of thumb. To demonstrate this, I will show a round robin of phase diagrams for fcc metals ($\ce{Ag}$, $\ce{Cu}$, $\ce{Au}$, $\ce{Ni}$) with no intermetallic compounds - just fcc solid and liquid. 1. $\ce{Ag}$-$\ce{Au}$, full mutual solubility, liquid and solid enthalpies of mixing pretty close: [](https://i.sstatic.net/6DiI1.png) 2. $\ce{Ag}$-$\ce{Cu}$, with limited mutual solid solubility and a eutectic: [](https://i.sstatic.net/PYV8V.png) 3. $\ce{Ag}$-$\ce{Ni}$, no solid solubility, a huge liquid miscibility gap: [](https://i.sstatic.net/qq2kn.png) 4. $\ce{Au}$-$\ce{Cu}$, complete mutual solid solubility plus a eutectic: [](https://i.sstatic.net/HnHfg.png) 5. $\ce{Au}$-$\ce{Ni}$, solid miscibility gap at lower temperatures, but complete solid miscibility above that, a slightly irregular liquidus: [](https://i.sstatic.net/4hGTp.png) 6. $\ce{Cu}$-$\ce{Ni}$, solid miscibility gap at lower temperatures, pretty ideal liquidus: [](https://i.sstatic.net/42KOJ.png) Bottom line: even for nominally 'simple' combinations of near-ideal fcc metals coming up with a workable rule of thumb just doesn't work.

Discussion on this answer:
Comment: After visualising a simplified version of your answer, I found this line: $\ce{Ag-Au-Cu-Ni}$. Metals on this line mix well with their neighbors. Maybe some real number parameter, like an $x$, could be ordered to them, and then we could say, they mix well if their $x$-parameters are close?
Comment: ...we could even append iron to the end of the list. Nickel mixes well with iron, but not with the others.
Comment: @peterh-ReinstateMonica - Indeed, Fe-Cu has limited solubility and a bit of an odd liquidus (nearly a small miscibility gap), Fe-Ag has a huge liquid solubility gap, and Fe-Au has a small eutectic and almost a range of complete solubility in the fcc phase across the composition range. Fe-Ni has complete fcc solubility, and even an ordered fcc low temperature phase.
Comment: There are about 75 experimentally observable metals in the periodic table. That means 2775 miscibility disagrams. Is it somewhere available? I think, some AI could find the most relevant and most simple ruleset quite easily.
Comment: ...it would not need even AI, simple gradient walking would be enough.
Comment: Well, the ASM (https://matdata.asminternational.org/apd/index.aspx) is the main keeper of all things for phase diagrams. The Calphad calculation method has lots of adherents, and a journal (and that is where my diagrams are generated from, out of ~1000 I've implemented).
Comment: I'd argue that structure of the pure elements is no simpler input than, for example, molar density and number of valence electrons of the elements. However, once all the binary phase diagrams are available, rules of thumb are not very practical.
Comment: @JonCuster Thanks. Unfortunately, it looks ASM would need a paid subscription what is not available for me in the case of hobby curiousity. I believe, the data should be made available for the whole public.
Comment: @peterh - well, your local research library will have books of phase diagrams in the reference section. The online is nicer, but lots of information is readily available.
Comment: @JonCuster Research library... nice to hear, but you know, last decades IT has taken over the brains here.
Comment: While, indeed, all journals at my institution are now online, there still exists the library (and librarians) and that includes reference works. Many of those, particularly the older ones, have not been digitized and remain available.
Comment: @JonCuster I think I could borrow it, scan it and then publish the scans? Thanks!


================================================================================

